Abstract
The electronic conductivities of ferroelectric domain walls have been extensively explored over the past decade for potential nanoelectronic applications. However, the realization of logic devices based on ferroelectric domain walls requires reliable and flexible control of the domainwall configuration and conduction path. Here, we demonstrate electricfieldcontrolled stable and repeatable onandoff switching of conductive domain walls within topologically confined vertex domains naturally formed in selfassembled ferroelectric nanoislands. Using a combination of piezoresponse force microscopy, conductive atomic force microscopy, and phasefield simulations, we show that onoff switching is accomplished through reversible transformations between charged and neutral domain walls via electricfieldcontrolled domainwall reconfiguration. By analogy to logic processing, we propose programmable logic gates (such as NOT, OR, AND and their derivatives) and logic circuits (such as fanout) based on reconfigurable conductive domain walls. Our work might provide a potentially viable platform for programmable allelectric logic based on a ferroelectric domainwall network with low energy consumption.
Similar content being viewed by others
Introduction
Domain walls (DWs) in ferroic materials have attracted intensive interest over the past decades due to their physical phenomena and potential for applications in nanoelectronics^{1,2} and spintronics^{3,4,5}. Of particular interest are the designs of racetrack memory^{6,7} and DW logic^{8,9} based on moving magnetic DWs driven by a current or a magnetic field. In these cases, data storage or logic operation functions could be realized by controlling DW injection, motion, and annihilation along magnetic nanowires rather than switching magnetic domains as is traditional. Contrary to the large wall width and high energy cost in currentdriven moving magnetic DWs, ferroelectric DWs possess a much smaller wall width (less than a few nanometers), and their electricfielddriven features and electric conduction are conducive to highdensity integration and lowpower regulation of nanoelectronic devices^{1,10,11,12,13,14,15,16,17,18,19,20,21,22,23,24,25}. Recently, by controlling the electric conduction of ferroelectric DWs with a low voltage, low or high resistance states could be created to realize 0 or 1 data bits for memory applications^{18,19,20,21,22,23,25}. For example, a prototype nonvolatile DW memory unit was demonstrated based on reconfigurable charged DWs (CDWs)^{19,20,21,23}, and the readout current of DWs hinged on the conformational changes of the DWs driven by an electric field between two inplane terminal electrodes. More intriguingly, ferroelectric DW memory was reported based on a highdensity CDW array with a controllable readout current^{18}.
Thus, CDWs can be used as dynamic functional entities, and their large local electric conduction also offers intriguing possibilities for potential nanometersized logic applications. Analogous to magnetic racetrack memory or DW logic in nanomagnetic, a ferroelectric DW diode and a fieldeffect transistor have recently been proposed. The former one is based on the unidirectional motion of all DWs in a terraced KTiOPO_{4} crystal lamella;^{26} the latter one is designed through erasing and rewriting of CDWs between the drain, gate, and source electrodes on a LiNbO_{3} single crystal^{25}. However, unlike magnetic DW logic in nanowires, the realization of ferroelectric DW logic is still a great challenge. The key issue is the implementation and integration of the CDW network with one CDW independently controlled without disturbing the other CDWs. Here, we demonstrate that CDWs within topologically confined vertex domains naturally formed in selfassembled BiFeO_{3} nanoislands^{18,27,28} can provide stable networks of local conductive paths for ferroelectric DW logic. Such a ferroelectric CDW network controllable by an electric field with nonvolatile conductance constitutes the building blocks for the proposed reconfigurable DW logic gates and circuits, indicating potential applications for allelectric memoryinlogic devices. By comparing with emerging magnetic DW devices^{6,7,8,9}, the ferroelectric DW logic units exhibit higher integration density due to a much smaller DW width, fast operating speed, and lower energy consumption due to the electricfielddriven features.
Results
Electric control of DW morphology and logic operation analogue
CDWs can naturally form in BiFeO_{3} nanoislands^{18,27,28,29,30}. By controlling the growth conditions (see “Methods”), we fabricated a BiFeO_{3} nanoisland array with a size of 200–350 nm and an aspect ratio of 1.0–1.5, as shown in Fig. 1a and Fig. S1. Piezoresponse force microscopy (PFM) and conductiveatomic force microscopy (cAFM) images (Fig. 1b, c and Fig. S2) show crossshaped CDWs of vertex domains confined in each nanoisland. The ferroelectric hysteresis loop (Fig. S3) and the corresponding PFM and cAFM images (Fig. S4) indicate the reversible control of the quaddomain between centerconvergent (Fig. S4a,b) and centerdivergent (Fig. S4d,e) polarization states, which accompanies with the headtohead CDWs with a low conductance state (~pA, Fig. S4c) and a tailtotail CWDs with a high conductance state (~nA, Fig. S4f)^{18}. For the headtohead CDWs in BiFeO_{3} nanoislands, the screening charges arise from the intrinsic electronic carriers (i.e., electrons liberated from oxygen vacancies) from ntype BiFeO_{3} nanoislands^{21,31}. While for the tailtotail CDWs, the screening charges arise from the ptype LSMO electrode when the quaddomain switched from a downward centerconvergent pattern to an upward centerdivergent pattern under the applied electric field, where a large number of holes are delivered to the tailtotail CDW region to compensate the negative bound charges^{18}.
To design ferroelectric DW logic based on CDWs, we first explore the dynamic behavior of the crossshaped CDWs with a high conductance state under a probebased trailing electric field^{13,32,33}. The details of the control process can be seen in Supplementary Fig. 5. Intriguingly, a targeted CDW of the offcenter vertex domains confined in a rectangular nanoisland with an aspect ratio deviating from 1 can be independently disconnected and connected again by a trailing electric field without affecting the other CDWs, as shown in Fig. 1d–f. For the initial state in Fig. 1d, the conductive paths of the four CDW branches of the offcenter vertex are connected. When an electric field of −3 V is applied on the nanoscale probe (Fig. S5a) with an inplane downward slowscanning direction (Fig. S5b), a trailing field along with the [\(\bar{1}\bar{1}0\)] direction is generated during probe scanning, and the targeted CDW branch is disconnected, as shown in Fig. 1e. This disconnected CDW can be reconnected by a trailing field along the [\(110\)] direction (Fig. S5c), as shown in Fig. 1f. The local current and the corresponding resistance state for the connected and disconnected CDW are recorded as shown in the lower panel of Fig. 1d–f. The reproducibility of the connection and disconnection of the CDW has been further confirmed by cAFM measurements (Fig. S6), and the corresponding low and high resistance state is also recorded as shown in Fig. S7. According to our previous results on the reversible control of the CDW resistance states on the vertex domains of nanoislands^{18}, the repeatable onandoff switching for CDW network could be no less than 10^{2} cycles. Moreover, time and temperaturedependent cAFM measurements, as shown in Figs. S8 and S9, respectively, also illustrate the stability of the modulated CDW network. Such robust control characteristics of the crossshaped CDWs of the offcenter vertex confined in the rectangular nanoisland allow reversible control of the ‘on’ and ‘off’ states of one CDW without interfering with the other CDWs. Notably, the CDWs in the square nanoisland with an aspect ratio of ~1.0 show negligible variation, e.g., the four CDWs remain after applying the inplane trailing field as shown in Fig. S10. This stability may arise from the topological protection of the square nanoisland^{18,30,34}.
Taking advantage of the reversible modulation of the local conductance states of the CDWs by a trailing field along with the [\(\bar{1}\bar{1}0\)] or [\(110\)] direction, we propose ferroelectric DW logic, as shown in Fig. 1g–i. The [\(\bar{1}\bar{1}0\)] and [\(110\)]oriented trailing fields are used to represent the input Boolean logic values ‘0’ and ‘1’, respectively, and the low and high conductance states between the two selected terminals of the crossshaped CDWs represent the output Boolean logic values ‘1’ and ‘0’, respectively. Here, the transistors are required to control which unit works and which does not, as shown in Fig. 1g, h. Thus, the switching between disconnected (Fig. 1e and g) and connected (Fig. 1f and h) CDWs by an electric field along with the [\(\bar{1}\bar{1}0\)] and [\(110\)]orientations, respectively, is analogous to a ‘NOT’ gate, as illustrated by the schematic and truth table in Fig. 1i.
Mechanism of connection and disconnection of ferroelectric DW
To understand the onandoff switching of the CDW, we performed phasefield simulations to investigate the evolution of the CDW configuration in a rectangular nanoisland under an inplane electric field (see Fig. 2a–c and Supplementary Movies 1, 2). Considering metals may be used as contacts in each of the proposed logic units, different screening charge densities were added to simulate the domain structures in the nanoisland, as shown in Fig. S11. As seen, the fourfold quaddomains remain either for the partially compensated state or for the fully compensated state. In Fig. 2, 156 μC/cm^{2} charges were added to 45° edges of the nanoisland, which means the inplane polarization induced bound charges have been fully compensated^{35}. The initial vertex state of the nanoisland (178 × 138 nm^{2}) shows centerdivergent quaddomains with a crossshaped CDW configuration (Fig. 2a). When an inplane [\(\bar{1}\bar{1}0\)]oriented electric field is applied in the area enclosed by a blue box in Fig. 2a, the pink area of the quaddomain with an inplane component of [\(\bar{1}\bar{1}0\)]oriented polarization grows, but the gray area of the quaddomain with an inplane component of [\(\bar{1}10\)]oriented polarization shrinks. This domain evolution is accompanied by DW bending (Fig. 2b), which drives the local DW to change from a CDW (Fig. 2d) to a neutral DW (Fig. 2e), as demonstrated by the transformation between crossshaped CDWs and interrupted DWs in the bound charge density map of Fig. 2g and h. The detailed definitions of the CDWs and neutral DWs can be seen in the inserts of Fig. 2d, e, and Supplementary Text. Due to the abrupt change in the bound charge density from a CDW to a neutral DW, as shown in the area enclosed by the blue box in Fig. 2g, h, the conductance is expected to dramatically decrease, which is consistent with the disconnected CDW in Fig. 1e. Intriguingly, if a [\(110\)]oriented electric field is applied in the area enclosed by the blue box in Fig. 2b, the disrupted CDW can be reoriented as shown in Fig. 2c, and transforms into a CDW, as demonstrated in Fig. 2f. The recovered high density of the bound charges for the CDW in Fig. 2i explains the reconnected CDWs in Fig. 1f. The corresponding intermediate domain images and the dynamic evolution for the CDWs from Fig. 2a to b, and Fig. 2b to c can also be seen in Supplementary Fig. 12 and Supplementary Movies 1 and 2, respectively. Additionally, we also performed phasefield simulations to investigate the reversible control of one CDW by the alternative [\(\bar{1}\bar{1}0\)] and [\(110\)]oriented electric field (Fig. S13), which is consistent with the experimental observation in Fig. 1d–f and Fig. S6.
The creation and annihilation of one CDW are related to the variation of the bound charge density during the polarization redistribution controlled by the external electric field. For the initial state in Fig. 2a, the orientation of the DW marked by the dashed box aligns along \([1\bar{1}0]\)crystalline orientation. In such cases, there are a large number of negative bound charges accumulated at the DW region (marked by ⊖ the symbol in Fig. 2d), which indicates the nanoisland with an initial CDW configuration with a high conductance state (Fig. 2g). After the application of [\(\bar{1}\bar{1}0\)]oriented electric field, the DW was bent nearly parallel to [\(010\)]orientation (Fig. 2b). In this case, the polarization vector rotated continuously across the DW region, resulting in a headtotail neutral DW (marked by ⊕ and ⊖ symbols in Fig. 2e), i.e., this segment changes from a CDW to a neutral DW (this segment CDW being annihilated). After applying a reversed electric field ([\(110\)]orientation), the DW was bent nearly to [\(\bar{1}\bar{1}0\)]orientation (Fig. 2c), where a great number of negative charges (marked by ⊖ symbol in Fig. 2f) accumulated at the DW region once again, resulting in a reversal change of this segment from a neutral DW to a CDW (this segment CDW being recreated, see Fig. 2i).
Design of NOR and NAND logic gates
Based on such robust control characteristics of the crossshaped CDWs of the offcenter vertex domains, more versatile logic gates (e.g., NOR and NAND) can be designed by connecting two rectangular nanoislands in parallel (Fig. 3) or series (Fig. S14). With two nanoislands combined in parallel, as shown in Fig. 3a, the electric fields (E1 and E2) used for control of the CDWs form the two logic inputs, and the conductance state, determined by the parallel resistance of the CDWs confined between the two selected terminals (green nodes), represents the logic output. To illustrate the functionality of the NOR gate, four different logic input configurations of ‘11’, ‘10’, ‘01’, and ‘00’ are illustrated in Fig. 3a–d, where the output conductance state is shown as ‘1’ (high resistance, HR) only when the investigated CDWs of the inparallel nanoislands are both disconnected; otherwise, it is shown as ‘0’ (low resistance, LR). The relationship between the logic inputs and outputs is summarized in Fig. 3e, which corresponds to the required logic operations for a NOR gate. To further illustrate the working principle of the proposed NOR gate with combined structures, a schematic of the crossbar structure is shown in Fig. S15. The input electric field for the upper panel nanoisland is implemented by Word line 1 (WL1) and WL2, and that for the lower panel nanoisland is implemented by WL3 and WL4, and the polarity of the electric field is controlled by the switching of the external circuit. The output resistance state is readout by Bit line 1 (BL1) and BL2. With two nanoislands connected in series, a NAND gate is implemented, as shown in Fig. S14. In this case, the output conductance state is shown as ‘0’ (LR) only when the investigated CDWs are both connected; otherwise, it is shown as ‘1’ (HR). Furthermore, the NAND gate can also be implemented when a third nanoisland serves as a Bias, as shown in Fig. S16.
Design of OR, AND, XOR, and XNOR logic gates
According to the ‘NOT’ logic gate illustrated in Fig. 1d–f, it is challenging to implement ‘1’ and ‘0’ logic outputs when the logic inputs are ‘11’ and ‘00’, respectively. While these logic operations are the essential ingredients for other basic logic gates, such as ‘OR’, ‘AND’, ‘XOR’, and ‘XNOR’. Thus, more versatile CDWs are needed to be explored, where the connection of one CDW and disconnection of another CDW are required concurrently when a unidirectional trailing field along [\(\bar{1}\bar{1}0\)] or [\(110\)]orientation is applied on one nanoisland. Accordingly, we explore the modulation of CDWs in a nanoisland with the size of 260 × 208 nm^{2} and AR of 1.25) as shown in Fig. 4a–c, where the initial four quaddomains show different symmetry compared with that of the above discussed four quaddomains. As can be seen in Fig. 4a, the cAFM image shows ~20 nA conductance at the CDW locations when the polarizations are upward and centerdivergent. The modulated CDWs by inplane trailing field are shown in Fig. 4b, c. When the inplane trailing field is along [\(\bar{1}\bar{1}0\)] direction, we observe that twoquarters of the DWs at the lower/upper panel are disconnected/connected (Fig. 4b), while what happens for the twoquarters of the DWs at the upper/lower panel when the inplane trailing field is along [\(110\)] direction (Fig. 4c). Thus, the high and low conductance states can be simultaneously implemented between \({A}^{{\prime} }\)/\({B}^{{\prime} }\) node and \({C}^{{\prime} }\)/\({D}^{{\prime} }\) node of the CDW network in Fig. 4b, as well as \({C}^{{\prime} }\)/\({D}^{{\prime} }\) node and \({A}^{{\prime} }\)/\({B}^{{\prime} }\) node in Fig. 4c, respectively. Taking advantage of such CDWs controlled by inplane downward and upward trailing fields in Fig. 4b, c, we design ‘OR’ and ‘AND’ logic gates by seriesconnected and parallelconnected two nanoislands with changeable DW networks as discussed above respectively, as shown in Fig. 4d–h and Fig. S17. In addition, other logic gates such as ‘XOR’ and ‘XNOR’ are also designed as shown in Figs. S18 and S19, respectively.
Digital signal readout and transmission by ferroelectric DW logic circuits
The demonstrations of the above logic gates make the concept of ferroelectric DW logic viable since any Boolean function can be implemented by combining these basic gates. Furthermore, signal readout and transmission, as schematically shown in the first column of Fig. 5, are also proposed based on an electricfieldcontrollable ferroelectric CDW network. For comparison, complementary metaloxide semiconductor (CMOS) and ferromagnetic DW logic circuits^{8} are also highlighted, as shown in the second and third columns of Fig. 5, respectively. For the signal readout, a low voltage and a high voltage can be read out directly at two ends (marked by black points) of a connected (the first panel of the fourth column in Fig. 5) and disconnected (the second panel of the fourth column in Fig. 5) CDW, and the readout signals can be easily switched between each other by an electric field (indicated by the bidirectional arrow in Fig. 5). The third panel of the fourth column of Fig. 5 shows a fanout circuit, where an input signal can be separated into two output signals of A and B. In this way, one might be able to integrate allelectric logic gates and circuits into the nanoisland array and regulate the function of each specific logic unit as needed.
Discussion
As discussed at the beginning, in comparison with emerging designs of racetrack memory and DW logic based on moving magnetic DW^{6,7,8,9}, the ferroelectric DW logic units exhibit higher integration density (Fig. S20) due to much smaller DW width and lower energy consumption due to electricfielddriven features. More comparison in the Supplementary Table 1 demonstrates some benefits of the ferroelectric DW logic circuit for device applications, such as low energy consumption, fast operation speed, and high integration density. For example, the operating energy for one bit estimated for the ferroelectric DW logic units is in 10 aJ order of magnitude, which is comparable to the emerging energyefficient magnetoelectric spinorbit logic but much lower than other emerging magnetic and existing CMOS technologies^{36}. Finally, it should be noted that the proposed ferroelectric DW logic units are preliminary designs and there are several challenges. For example, the endurance of the CDW network under electric fielddriven repeated onandoff switching (Figs. 1d–f) and operation at higher temperatures (Fig. S9) remain to be improved. One possible way to address this issue in the future is to design the geometry (size and AR) of the nanoislands^{30,37}, such that the shape and thickness of the CDW might be accurately confined by the symmetry of the nanoislands. Another big challenge is the logic cascading of the single logic gates, which may be implemented by appropriate circuit design and connection, e.g., the voltage corresponding to the resistance state of the DW can be set as output, and then the output voltage can be used as the input of the next logic gate, to achieve cascade.
In summary, we demonstrate electricfield controlled stable and repeatable onandoff switching of conductive domain walls within topologically confined vertex domains naturally formed in selfassembled ferroelectric nanoislands, which is accompanied by the transformations between charged and neutral domain walls via electricfield controlled domainwall reconfiguration. By analogous to logic processing, we also propose programmable logic gates and circuits based on reconfigurable conductive domain walls. This ferroelectric memoryinlogic architecture proposed based on the flexible control of conducting domainwall network might allow for designing programmable allelectric logic with low energy consumption.
Methods
Preparation of ferroelectric nanoisland array with CDWs
BiFeO_{3} thin films were prepared by pulsed laser deposition method on LaAlO_{3} (001) singlecrystal substrates, where a very thin (2 nm) (La,Sr)MnO_{3}(LSMO) buffer layer was pregrown to construct the required electrostatic and elastic boundary conditions for the nucleation of selfassembled BiFeO_{3} nanoislands. During the thinfilm preparation, the growth temperature was maintained in the range of 600–750 °C under the oxygen pressure of 0.2 mbar. The growth details for BiFeO_{3} nanoisland array are similar to our previous work^{27}.
PFM measurements for ferroelectricdomain configurations
The polar vectors of the threedimensional BiFeO_{3} nanoislands were investigated by the combination of vertical and lateral PFM phase images using an Infinity Asylum Research AFM and a Bruker AFM. During the measurement, a commercial Pt/Ircoated tip with a tip radius of 20 nm, a force constant of 2.8 N/m, and a resonant frequency of 75 kHz was used as a movable top electrode, where the bottom electrode (LSMO layer) was ground. The PFM signal was collected at the contact resonance frequency with an a.c. tip bias of 1 V_{pp}, and the scanning velocity of the cantilever is 0.5 μm/s.
cAFM measurements for conducting DW network
The conductance of the BiFeO_{3} nanoislands was characterized by cAFM, which is also based on an Infinity Asylum Research AFM and a Bruker AFM. In the cAFM model, a commercial Pt/Ircoated tip was used. During the conductance measurement, the tip was ground and the voltage bias was applied to the LSMO bottom electrode. The bias voltage applied to the LSMO bottom electrode is ~1.5 V.
Phasefield simulations
Phasefield simulations were carried out using the timedependent GinzburgLandau model for the investigation of domain evolution and DW network in BiFeO_{3} nanoislands. Ferroelectric polarization evolution is described by the polarization vector \({{{{{{\bf{P}}}}}}}_{i}\)(\({P}_{x}\), \({P}_{y}\), \({P}_{z}\)), which is the order parameter to describe the domain structure. The model describes the temporal evolution of domain structure, which can be numerically solved by the timedependent LandauGinzburg (TDGL) equation,
where t, L, and F_{p} are simulation time, kinetic coefficient (related to DW mobility), and total free energy respectively, whereas:
where f_{bulk}, f_{grad}, f_{elas}, and f_{elec} are bulk free energy density^{38}, gradient energy density, elastic energy density, and electric energy density^{39}, respectively. The bulk free energy density f_{bulk} is a sixthorder polynomial,
where \({\alpha }_{1},{\alpha }_{11},{\alpha }_{12},{\alpha }_{111},{\alpha }_{112}\) and \({\alpha }_{123}\) are dielectric stiffness and high order stiffness. Among them, only \({\alpha }_{1}\) depends on the temperature, such that \({\alpha }_{1}\) = (T−T_{0})/(2ε_{0}C_{0}), T is temperature, T_{0} is Curie temperature, ε_{0} = 8.85 × 10^{−12 }F/m is dielectric permittivity of vacuum, C_{0} is the Curie constant.
The gradient energy density is described in terms of polarization gradients. For simplicity, the gradient energy is taken to be isotropic, given as:
where the \({g}_{{ijkl}}\) is gradient energy coefficient and \({{{{{{\bf{P}}}}}}}_{i.j}=\partial {P}_{i}/\partial {x}_{j}\)^{40}\(.\) The elastic energy can be written as,
where the \({c}_{{ijkl}}\) is elastic stiffness tensor, \({e}_{{ij}}\) is elastic strain, \({\varepsilon }_{{ij}}\) is total elastic strain, \({\varepsilon }_{{ij}}^{0}\) is the stressfree strain given as \({\varepsilon }_{{ij}}^{0}={Q}_{{ijkl}}{P}_{k}{P}_{l}\), where \({Q}_{{ijkl}}\) represents the electrostrictive coefficient^{41}. The electrostatic energy, \({f}_{{{\mbox{elec}}}}\), is given by,
In the present simulations, an open circuit boundary condition with fully compensated edge charges (156 μC/cm^{2}) on edge tilts and chargefree on the substrate and top surface was used as an electrostatic boundary condition, and a strainfree mechanical boundary condition was used at the working temperature of 300 K. The nanoisland was constructed with a size of 178 nm × 138 nm at the base and 7 nm at the island height, and the edge tilt was taken as 45° for the simulations. The value of coefficients used for the current work is listed in Supplementary Table 2^{42}. The parameters of permittivity and Curie constant (C_{0}) used in the phasefield simulations are 50 and 1.2166 × 10^{5 }K, respectively.
Reporting summary
Further information on research design is available in the Nature Research Reporting Summary linked to this article.
Data availability
The authors declare that the data supporting the findings of this study are available within the paper and its Supplementary Information Files.
References
Catalan, G., Seidel, J., Ramesh, R. & Scott, J. F. Domain wall nanoelectronics. Rev. Mod. Phys. 84, 119–156 (2012).
Meier, D. & Selbach, S. M. Ferroelectric domain walls for nanotechnology. Nat. Rev. Mater. 7, 157–173 (2022).
Yang, S.H., Naaman, R., Paltiel, Y. & Parkin, S. S. P. Chiral spintronics. Nat. Rev. Phys. 3, 328–343 (2021).
Raymenants, E. et al. Nanoscale domain wall devices with magnetic tunnel junction read and write. Nat. Electron. 4, 392–398 (2021).
Li, R. et al. A spin–orbit torque device for sensing threedimensional magnetic fields. Nat. Electron. 4, 179–184 (2021).
Parkin, S. S. P., Hayashi, M. & Thomas, L. Magnetic domainwall racetrack memory. Science 320, 190–194 (2008).
Thomas, L., Moriya, R., Rettner, C. & Parkin, S. S. P. Dynamics of magnetic domain walls under their own inertia. Science 330, 1810–1813 (2010).
Allwood, D. A. et al. Magnetic domainwall logic. Science 309, 1688–1692 (2005).
Luo, Z. et al. Currentdriven magnetic domainwall logic. Nature 579, 214–218 (2020).
Sluka,T., Bednyakov, P., Yudin, P., Crassous, A. & Tagantsev, A. in Topological Structures in Ferroic Materials: Domain Walls, Vortices and Skyrmions (ed. Seidel, J.) 103–138 (Springer International Publishing, 2016).
Seidel, J. Domain walls in motion. Nat. Nanotechnol. 10, 109 (2015).
Seidel, J. et al. Conduction at domain walls in oxide multiferroics. Nat. Mater. 8, 229–234 (2009).
Crassous, A., Sluka, T., Tagantsev, A. K. & Setter, N. Polarization charge as a reconfigurable quasidopant in ferroelectric thin films. Nat. Nanotechnol. 10, 614–618 (2015).
McGilly, L. J., Yudin, P., Feigl, L., Tagantsev, A. K. & Setter, N. Controlling domain wall motion in ferroelectric thin films. Nat. Nanotechnol. 10, 145–150 (2015).
Rojac, T. et al. Domainwall conduction in ferroelectric BiFeO3 controlled by accumulation of charged defects. Nat. Mater. 16, 322–327 (2017).
Lu, H. et al. Electrical tunability of domain wall conductivity in LiNbO_{3} thin films. Adv. Mater. 31, 1902890 (2019).
Zhang, Y. et al. Intrinsic conductance of domain walls in BiFeO_{3}. Adv. Mater. 31, 1902099 (2019).
Ma, J. et al. Controllable conductive readout in selfassembled, topologically confined ferroelectric domain walls. Nat. Nanotechnol. 13, 947–952 (2018).
Jiang, J. et al. Temporary formation of highly conducting domain walls for nondestructive readout of ferroelectric domainwall resistance switching memories. Nat. Mater. 17, 49–56 (2018).
Jiang, A. Q. et al. Ferroelectric domain wall memory with embedded selector realized in LiNbO_{3} single crystals integrated on Si wafers. Nat. Mater. 19, 1188–1194 (2020).
Sharma, P. et al. Nonvolatile ferroelectric domain wall memory. Sci. Adv. 3, e1700512 (2017).
McConville, J. P. V. et al. Ferroelectric domain wall memristor. Adv. Funct. Mater. 30, 2000109 (2020).
Sharma, P. et al. Conformational domain wall switch. Adv. Funct. Mater. 29, 1807523 (2019).
Liu, L. et al. Giant domain wall conductivity in selfassembled BiFeO_{3} nanocrystals. Adv. Funct. Mater. 31, 2005876 (2020).
Chai, X. et al. Nonvolatile ferroelectric fieldeffect transistors. Nat. Commun. 11, 2811 (2020).
Whyte, J. R. & Gregg, J. M. A diode for ferroelectric domainwall motion. Nat. Commun. 6, 7361 (2015).
Ma, J. et al. Selfassembly growth of a multiferroic topological nanoisland array. Nanoscale 11, 20514–20521 (2019).
Kim, K. E. et al. Configurable topological textures in strain graded ferroelectric nanoplates. Nat. Commun. 9, 403 (2018).
Li, Z. et al. Highdensity array of ferroelectric nanodots with robust and reversibly switchable topological domain states. Sci. Adv. 3, e1700919 (2017).
Ma, J. et al. Geometry confined polar vertex domains in selfassembled BiFeO_{3} nanoislands. Mater. Res. Lett. 7, 399–404 (2019).
Wu, W., Horibe, Y., Lee, N., Cheong, S.W. & Guest, J. R. Conduction of topologically protected charged ferroelectric domain walls. Phys. Rev. Lett. 108, 077203 (2012).
Vasudevan, R. K. et al. Deterministic arbitrary switching of polarization in a ferroelectric thin film. Nat. Commun. 5, 4971 (2014).
Wang, C. et al. Ferroelastic switching in a layeredperovskite thin film. Nat. Commun. 7, 10636 (2016).
Chen, M. et al. Stabilization of ferroelastic charged domain walls in selfassembled BiFeO_{3} nanoislands. J. Appl. Phys. 128, 124103 (2020).
Chu, Y.H., Martin, L. W., Holcomb, M. B. & Ramesh, R. Controlling magnetism with multiferroics. Mater. Today 10, 16–23 (2007).
Manipatruni, S. et al. Scalable energyefficient magnetoelectric spin–orbit logic. Nature 565, 35–42 (2018).
Chen, M. et al. Robust polarization switching in selfassembled BiFeO3 nanoislands with quaddomain structures. Acta Materialia 175, 324–330 (2019).
Li, Y. L., Hu, S. Y., Liu, Z. K. & Chen, L. Q. Phasefield model of domain structures in ferroelectric thin films. Appl. Phys. Lett. 78, 3878–3880 (2001).
Li, Y. L., Hu, S. Y., Liu, Z. K. & Chen, L. Q. Effect of electrical boundary conditions on ferroelectric domain structures in thin films. Appl. Phys. Lett. 81, 427–429 (2002).
Pertsev, N. A., Kukhar, V. G., Kohlstedt, H. & Waser, R. Phase diagrams and physical properties of singledomain epitaxial PbZr(1x)TixO_{3} thin films. Phys. Rev. B 67, 054107 (2003).
Haun, M. J., Furman, E., Jang, S. J., Mckinstry, H. A. & Cross, L. E. Thermodynamic theory of PbTiO_{3}. J. Appl. Phys. 62, 3331–3338 (1987).
Hsieh, Y.H. et al. Permanent ferroelectric retention of BiFeO_{3} mesocrystal. Nat. Commun. 7, 13199 (2016).
Acknowledgements
We thank Dr. X.M. Shi for his discussion on logic operations. We are also grateful to Analysis & Testing Center at BIT. This work was supported by the Basic Science Center Program of the National Natural Science Foundation of China (NSFC) grant 51788104; NSFC grant 12004036, 51922055, 51972028, 52002204, and 11974052; and the National Basic Research Program of China grant 2019YFA0307900.
Author information
Authors and Affiliations
Contributions
C.W.N. conceived the project. J.W., Jing M., H.H., and D.Y. performed the logic study. Ji M. and M.C. fabricated the thin films. J.W., Ji M., Y.F., H.Y., and Y.W. performed PFM and cAFM measurements. H.J. and D.L. performed the phasefield simulations under the supervision of H.H. and L.Q.C. J.W., H.H., and Jing M. wrote the draft of the manuscript. J.Z. and Y.L. discussed the results. All authors discussed the results and edited the manuscript.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing interests.
Peer review
Peer review information
Nature Communications thanks Cheol Seong Hwang and the other anonymous reviewer(s) for their contribution to the peer review of this work.
Additional information
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Wang, J., Ma, J., Huang, H. et al. Ferroelectric domainwall logic units. Nat Commun 13, 3255 (2022). https://doi.org/10.1038/s41467022309834
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s41467022309834
This article is cited by

Formation and energetics of headtohead and tailtotail domain walls in hafnium zirconium oxide
Scientific Reports (2024)

Machine learning surrogate for 3D phasefield modeling of ferroelectric tipinduced electrical switching
npj Computational Materials (2024)

Electricfieldinduced crystallization of Hf0.5Zr0.5O2 thin film based on phasefield modeling
npj Quantum Materials (2024)

A review on different theoretical models of electrocaloric effect for refrigeration
Frontiers in Energy (2023)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.